International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 08  Aug 2018
pISSN: 23950072
www.irjet.net
Parametric optimization of submerged arc welding process by using Response Surface Methodology N.D.Jadhav1, Bipin Diwakar2, Prasad Shinde3 1Assistant
Professor , Mechanical Department , Ashokrao Mane Group Of Institutions, Vatahar, Kolhapur, India. Mechanical Department , Ashokrao Mane Group Of Institutions, Vatahar, Kolhapur, India.
2,3Student,
***
Abstract : Submerge arc welding (SAW) has become a natural choice in industries for fabrication, especially for welding of pipes because of its deep penetration, smooth finish and high productivity. Optimum ranges of bead parameters are required for better economy and to ensure the desired mechanical properties. The above objectives can easily be achieved by development of mathematical model and execution of the experiments by response surface methodology. Response surface methodology (RSM) is a technique to determine and represent the cause and effect relationship between true mean responses and input control variables influencing the responses as a two or three dimensional hyper surface. This paper highlights the use of (RSM) by designing a fourfactor twolevel design matrix for planning, execution and development of mathematical model. For Experiment [SA516 (Gr70)] is used as a base metal. Main and interaction effects of the process variables on bead geometry and shape factors are presented in graphical form. From the experimental results, it is found that speed and voltage plays major role in finding weld bead dimensions. . IndexTerms :SAW, optimization, Regression analysis, Response surface methodology, weld bead geometry INTRODUCTION The submerged arc welding process is often preferred because it offers high production rate, high melting efficiency, ease of automation and low operator skill requirement.[4] the desired welding parameters are obtained based from charts or handbook value which are difficult cumbersome and they does not ensure that chosen welding parameters are optimal for particular welding environmental.[1]Even smaller change in the welding process parameters may causes unexpected welding performance. Therefore, it is important to study stability of welding parameters to achieve high quality welding. [5] Optimum process parameters selection has been investigated by some significant studies via establishing a mathematical model correlating welding parameters with quality characteristics using different approaches [1]In this study, mathematical relations (empirical equations) between submerged arc welding process parameters and weld bead characteristics were constructed based upon the experimental data obtained by four parameterstwo levels factorial analysis. The empirical equations, simulating the submerged arc welding process approximately, were carried out by Multiple Regression Analysis and sensitivity equations were derived from these basic models. An analysis generally requires a definition of an objective function and design parameters. In this study, the objective function (quality function) was chosen as weld bead characteristics (the width, height of the weld bead) whereas process parameters (arc current, voltage, welding speed and stickout) were selected as the design variables. The present study mainly focuses on the determination of sensitivity characteristics of design parameters and the prediction of finetuning requirements, of these parameters in submerged arc welding process. The results revealed considerable information about process parameter tendencies and optimum welding conditions appearance and the absence of any visible defects. For deciding the working range, several trial welds were made. For determining the range of one variable, the other three variables were kept constant during trial runs. A similar procedure was adopted for determining the upper and lower limits for the welding speed and nozzletoplate distance. Also, trial welds were made, keeping the values of all the parameters both at their minimum and maximum values to were kept constant during trial runs. A similar procedure was adopted for determining the upper and lower limits for the welding speed and nozzletoplate distance. Also, trial welds were made, keeping the values of all the parameters both at their minimum and maximum values to verify quality of the weld bead, after determining the working range of the process parameters, the upper limit was coded as +1 and 1 After determining the working range of the process parameters ,the upper limit was coded as +1 and lower limit as 1.The coded value of the intermediate levels were calculated from the relationship[49] Xi=2 xâˆ’(Xmax+Xmin)/(Xmaxâˆ’Xmin) Where Xi the required coded value of a variable X; and X is is any value of the variable from X min to X max. .
ÂŠ 2018, IRJET

Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 1093
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 08  Aug 2018
pISSN: 23950072
www.irjet.net
3.DEVELOPING THE DESIGN MATRIX: The selected design matrix, shown in Table 2, factorial design [4] consisting of 16 sets of coded conditions. Design matrix is blocked with their result to reduce irrelevant source of variation. Response variables bead width and reinforcement are measured by using scale and venire caliper. The selected process parameters with their limits, units and notations are given. Cross sectional picture of weld bead is given below.
Fig:1CrossSectional of weld bead, where W be weld width in mm, R be the Reinforcement in mm. 4.DEVELOPMENT OF MATHEMATICAL MODEL: The response function representing any of the weld bead dimensions can be expressed as [29] Y=F(S, V, I, N) Where Y is the response (Bead width, reinforcement) I is the welding currents, amps S is the welding speed, Inch/min. N is the nozzle to plate distance, mm. The relationship selected being a First degree response surface expressed as follows: Y=B0+B1X1+B2X2+.............+BKXK+ε 5.CHECKING THE ADEQUACY OF THE MODELS DEVELOPED: The adequacy of the models was tested using the analysisofvariance technique (ANOVA). As per this technique [27]: The estimated coefficients obtained above were used to construct models for the response parameters. The adequacy of the models so developed was then tested by using the analysis of variance technique (ANOVA). Using this technique, it was found that calculated F ratios were larger than the tabulated values at a 95% confidence level; hence, the models are considered to be adequate The adequacy of a fitted regression model are the coefficient of determination (R'). For the models developed, the calculated R2 and adjusted R2 values were above 80% and 70%, respectively. These values indicate that the regression models are quite adequate the validity of regression models developed were further tested by drawing scatter diagrams.The observed values and predicted values of the responses are scattered close to the 45 ° line, indicating an almost perfect fit of the developed empirical models. To improve the reliability of result, experiment were planned on the basis of response surface methodology (RSM) techniques for statistical design of experiment. 6.EXPERIMENTAL SET UP : The equipment is conducted on ESAB submerged arcwelding equipment.EH14, 2. 4mm diameter of welding rods are used. SA516 Gr70 steel plates of 500mm× 150mm×12mm size are selected as a working material and bead on joint with single V butt joint with 0.5–1mm root gap is consider.Flux: ADOR make F7P2 granular type is used.
© 2018, IRJET

Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 1094
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 08  Aug 2018
pISSN: 23950072
www.irjet.net
Fig:2 ESAB Submerged Arc Welding Machine 7.Response Surface Methodology: RSM is sequential procedure often when we are at a point on the response surface that is remote from the optimum; our object here is to lead the experimenter rapidly and efficiently along a path of improvement towards the general vicinity of the optimum. Once the region of the optimum has been found a more elaborate model such as secondorder model may be employed& an analysis may be performed to locate optimum. The eventual object of RSM is to determine the optimum operating conditions for the system or to determine a region of the factor space in which operating requirements are satisfied. chemical composition of work piece is given below. Table 1 Chemical composition of work piece (SA516 Gr: 70) Carbon
Manganese
Phosphorus max4
Sulfur max4
Silicon
0.27
0.791.30
0.035
0.035
0.130.45
Process parameters and their limits are given below. Table: 2. Process control parameters and their limits Variables
Natural Value
Speed Voltage Current
20 32 30 0 22
Distance
24 40 360
Coded Value 1 1 1
+1 +1 +1
25
1
+1
Coded design matrix of weldments are given below. Table: 3. Coded design matrix of weldments Weld
Block I
conditions
Sp
Vot
Cu
Dis
Rein
1
1
1
1
1
4
1
1
1
6
1
1
7
1
1
ÂŠ 2018, IRJET

Weld
Block II
Width
Cindition
Sp
Vot
Cu
Dis
Rein
Width
1.5
20.02
2
1
1
1
1
1.3
17.66
1
1.0
18.42
5
1
1
1
1
1.6
20
1
1
2.4
18.1
8
1
1
1
1
1.8
19
1
1
1.4
18.6
9
1
1
1
1
1.2
19.26
Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 1095
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 08  Aug 2018
pISSN: 23950072
www.irjet.net
10
1
1
1
1
1.9
18.14
11
1
1
1
1
2.1
18.54
11
1
1
1
1
2.1
18.20
12
1
1
1
1
1.4
18.08
13
1
1
1
1
2.0
17.60
14
1
1
1
1
2
18.06
16
1
1
1
1
1.9
19.20
15
1
1
1
1
2.2
18.60
7.1Regression Analysis [With blocking] the regression equation for BlockI is Reinforcement2 = 1.780.0250sp20.150 vol2+0.200cu2+0.325dis2 Table 5 Significance table Predictor
Coef
SE coef
T
P
Constant
1.77500
0.04330
40.99
0.000
Sp2
0.02500
0.04330
0.58
0.604
Vol2
0.1500
0.04330
3.46
0.041
Cu2
0.20000
0.04330
4.62
0.019
Distance2
0.32500
0.04330
7.51
0.005
S=0.122474 RSq=96.8% RSQ(adj)=92.5% Then the regression equation for BlockII is Reinforcement3=1.700.225sp30.100vol3+0.100cu3+0.225dis3 Table 5.1Significance table Predictor
Coef
SE Coef
T
P
Constant
1.70000
0.04564
37.25
0.000
Sp3
0.22500
0.04564
4.93
0.016
Vol3
0.10000
0.04564
2.19
0.116
Cu3
0.10000
0.04564
2.19
0.116
Dist3
0.22500
0.04564
4.93
0.016
S=0.129099 R2=95.1% RSQ(adj)=88.6% By comparing First block and second block it is seen that Voltage, Current, distance is significant and its RSq=96.8% RSQ(adj)=92.5%,whereas in blockII Speed and distance is significant whereas its R2=95.1% RSQ(adj)=88.6% so comparing Block I and BlockII, BlockI gives better results so further result analysis is done with BlockI ,and scatterplot of reinforcement verses nozzle to plate distance and voltage are given below.
ÂŠ 2018, IRJET

Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 1096
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 08  Aug 2018
pISSN: 23950072
www.irjet.net
Fig3:Scatterplot of reinforcement Vs distance between plate and nozzle.and Scatterplot of reinforcement Vs voltage.
Fig4:Scatter plot of reinforcementVs Speed
Fig5:Surface plot of reinforcement Vs speed, voltage.
Fig:6 Surface plot of reinforcement Vs current, distance
ÂŠ 2018, IRJET

Impact Factor value: 7.211

Fig:7Surface plot of reinforcement Vs speed, distance
ISO 9001:2008 Certified Journal

Page 1097
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 08  Aug 2018
pISSN: 23950072
www.irjet.net
Fig:7 Optimization Plot for Reinforcement.
Fig:8 Optimization Value for Reinforcement 7.2.1Optimization Value for Reinforcement Conduction of Experiments by considering optimality loss the optimise value becomes Table 5.4 Reinforement table
ÂŠ 2018, IRJET
Voltage
Current
Distance
Reinforcement
32
340
25
2.3

Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 1098
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 08  Aug 2018
pISSN: 23950072
www.irjet.net
7.2.2 Scatter plot for width verses current,Voltage and nozzle to plate distance are given below.
Fig:9 Scatterplot of width Vs Voltage.
Fig:10 Surface plot of width Vs Current.
Fig:11 Scatterplot of width Vs distance.
ÂŠ 2018, IRJET

Impact Factor value: 7.211
Fig12:Surface plot of width Vs speed, voltage.

ISO 9001:2008 Certified Journal

Page 1099
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 08  Aug 2018
pISSN: 23950072
www.irjet.net
Fig13:Optimum Value for Width
Fig14:Optimization Plot for Width
Â© 2018, IRJET

Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 1100
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 08  Aug 2018
pISSN: 23950072
www.irjet.net
7.2.3 Optimum value for width. Conduction of Experiments by considering optimality loss the optimise value becomes Voltage
Current
Width
20
32
18
8 Results: Mathematical model is used to predict the weld bead geometry by substituting the values in the coded form of the respective factors. The responses calculated from these models for each set of coded welding variable in graphical form .Substituting the values of the desired bead geometry, the value of the control factor in coded form can be obtained. In general the result show convincing trends between cause & the effect. 8.1.1 Direct effect of the process parameters •
As the voltage increases reinforcement decreases and Bead width increases.
•
As the current increases reinforcement and bead width increases.
•
.As the speed increases reinforcement decreases
•
As the stick out increases reinforcement is increases and bead width decreases
8.1.2Interaction Effect on reinforcement & bead width: • Speed and Voltage on Reinforcement: Combined effect of speed and voltage is shown in figure 5. from figure it is clear that, Reinforcement gradually decreases with increases in speed, as speed is increased heat input per length of weld is decreased, Due to that weld deposition is smaller so as the Speed increases reinforcement and width also decreases. As voltage increased reinforcement decreased, because voltage is directly to the length of the current path between the welding wire and workpiece.so as the stickout increases voltage is also increases, due to that bead width is gradually increases and reinforcement is decreases. . • Current and stickout on reinforcement: Combined effect of current and stickout on reinforcement is shown in figure 6.From figure it is clear that, As the current increases reinforcement Increases. Too high current also means waste of power & waste of welding wire in the form of reinforcement .if the current is too low then there is insufficient reinforcement occurred where as stickout having positive effect on reinforcement. • Speed and Stickout on Reinforcement: Combined effect of speed and stickout on reinforcement is shown in figure 7. From figure it is clear that, Reinforcement Gradually decreases with increases in speed. But as the stickout increases reinforcement gradually increases so from this it is clear that speed having negative result on reinforcement where as stickout having positive effect on reinforcement. As the speed is increased heat input per length of weld is decreased, due to that weld deposition is smaller so as the Speed increases reinforcement decreases. • Speed and Voltage on width: Combined effect of speed and voltage on width is shown in figure 12. From figure it is clear that, Voltage is having Positive effect on bead width and Speed having Negative effect on width. Width is gradually decreases with increases in speed, as speed is increased heat input per length of weld is decreased, Due to that weld deposition is smaller so as the Speed increases width and reinforcement also decreases. As voltage is directly to the length of the current path between the welding wire and workpiece.so as the stickout increases voltage is also increases, due to that bead width is gradually increases References [1] Benyounis K.Y, Olabi A.G, Optimization of different welding processes using statistical and numerical approaches – A reference guide, Advances in Engineering Software 39 (2008) 483–496 [2] Palani P.K. Murgan.N, Sensitivity Analysis for process parameters in Cladding of Stainless Steel by flux cored arc welding, Journal of Manufacturing Processes Vol. 8/No. 2 2006
© 2018, IRJET

Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 1101
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 08  Aug 2018
pISSN: 23950072
www.irjet.net
[3] Karaoglu Serdar, Secgin Abdullah, Sensitivity analysis of submerged arc welding process parameter, Journal of material process technology 202(2008)500507 [4] Gunaraj V, Murugan N, Application of response surface methodology for predicting weld bead quality in submerged arc welding of pipes, Journal of Materials Processing Technology 88 (1999) 266–275 [5] Gunaraj V, Murugan N, Prediction and comparison of the area of the heataffected zone for the beadonplate and beadonjoint in submerged arc welding of pipes, Journal of Materials Processing Technology 95 (1999) 246261 [6] Design and analysis of experiment book by Douglas Montgomery [7]Murugan N,Gunaraj V, Prediction and control of bead geometry and shape relationships in submerged arc welding of pipes, Journal of Materials Processing Technology 168 (2005) 478487 [8]Nowacki Jerzy, Rybicki Pawel, The influence of welding heat input on submerged arc welded duplex steel joints imperfections, Journal of Materials Processing Technology 164–165 (2005) 1082–1088 [9]Patnaik Amar, Biswas Sandhyarani, Mahapatra S.S., An evolutionary approach to parameter optimisation of submerged arc welding in the hard facing process, Int. J. Manufacturing Research, Vol. 2, No. 4, 2007
© 2018, IRJET

Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 1102
https://www.irjet.net/archives/V5/i8/IRJETV5I8190.pdf
Published on Sep 14, 2018
https://www.irjet.net/archives/V5/i8/IRJETV5I8190.pdf